Resistive random-access memory
|This article's lead section may not adequately summarize key points of its contents. (August 2014)|
|Computer memory types|
|Early stage NVRAM|
Resistive random-access memory (RRAM or ReRAM) is a type of non-volatile (NV) random-access (RAM) computer memory that works by changing the resistance across a dielectric solid-state material often referred to as a memristor. This technology bears some similarities to conductive-bridging RAM (CBRAM), and phase-change memory (PCM).
CBRAM involves one electrode providing ions that dissolve readily in an electrolyte material, while PCM involves generating sufficient Joule heating to effect amorphous-to-crystalline or crystalline-to-amorphous phase changes. On the other hand, RRAM involves generating defects in a thin oxide layer, known as oxygen vacancies (oxide bond locations where the oxygen has been removed), which can subsequently charge and drift under an electric field. The motion of oxygen ions and vacancies in the oxide would be analogous to the motion of electrons and holes in a semiconductor.
RRAM is currently under development by a number of companies, some of which have filed patent applications claiming various implementations of this technology. RRAM has entered commercialization on an initially limited KB-capacity scale.
Although anticipated as a replacement technology for flash memory, the cost benefit and performance benefit of RRAM have not been enough for companies to proceed with the replacement. A broad range of materials apparently can potentially be used for RRAM. However, the discovery that the popular high-κ gate dielectric HfO2 can be used as a low-voltage RRAM has greatly encouraged others to investigate many other possibilities. Among others, SiOx has been identified to offer significant benefits. Weebit-Nano Ltd is one company that is pursuing SiOx and has already demonstrated functional devices.
In February 2012 Rambus bought an RRAM company called Unity Semiconductor for $35 million. Panasonic launched an RRAM evaluation kit in May 2012, based on a tantalum oxide 1T1R (1 transistor – 1 resistor) memory cell architecture.
In 2013, Crossbar introduced an RRAM prototype as a chip about the size of a postage stamp that could store 1 TB of data. In August 2013, the company claimed that large-scale production of their RRAM chips was scheduled for 2015. The memory structure (Ag/a-Si/Si) closely resembles a silver-based CBRAM.
Different forms of RRAM have been disclosed, based on different dielectric materials, spanning from perovskites to transition metal oxides to chalcogenides. Silicon dioxide was shown to exhibit resistive switching as early as 1967, and has recently been revisited.
Leon Chua argued that all two-terminal non-volatile memory devices including RRAM should be considered memristors. Stan Williams of HP Labs also argued that RRAM was a memristor. However, others challenged this terminology and the applicability of memristor theory to any physically realizable device is open to question. Whether redox-based resistively switching elements (RRAM) are covered by the current memristor theory is disputed.
In 2014 researchers announced a device that used a porous silicon oxide dielectric with no edge structure. In 2010 conductive filament pathways were discovered, leading to the later advance. It can be manufactured at room temperature and has a sub-2V forming voltage, higher on-off ratio, lower power consumption, nine-bit capacity per cell, higher switching speeds and improved endurance.
The basic idea is that a dielectric, which is normally insulating, can be made to conduct through a filament or conduction path formed after application of a sufficiently high voltage. The conduction path can arise from different mechanisms, including vacancy or metal defect migration. Once the filament is formed, it may be reset (broken, resulting in high resistance) or set (re-formed, resulting in lower resistance) by another voltage. Many current paths, rather than a single filament, are possibly involved. The presence of these current paths in the dielectric can be in situ demonstrated via conductive atomic force microscopy.
The low-resistance path can be either localized (filamentary) or homogeneous. Both effects can occur either throughout the entire distance between the electrodes or only in proximity to one of the electrodes. Filamentary and homogenous switching effects can be distinguished by measuring the area dependence of the low-resistance state.
Under certain conditions, the forming operation may be bypassed. It is expected that under these conditions, the initial current is already quite high compared to insulating oxide layers.
CBRAM cells generally would not require forming if Cu ions are already present in the electrolyte, having already been driven-in by a designed photo-diffusion or annealing process; such cells may also readily return to their initial state. In the absence of such Cu initially being in the electrolyte, the voltage would still be applied directly to the electrolyte, and forming would be a strong possibility.
For random-access type memories, a 1T1R (one transistor, one resistor) architecture is preferred because the transistor isolates current to cells that are selected from cells that are not. On the other hand, a cross-point architecture is more compact and may enable vertically stacking memory layers, ideally suited for mass-storage devices. However, in the absence of any transistors, isolation must be provided by a "selector" device, such as a diode, in series with the memory element or by the memory element itself. Such isolation capabilities are inferior to the use of transistors if the on/off ratio for the selector is not sufficient, limiting the ability to operate very large arrays in this architecture. Thin film based threshold switch can work as a selector for bipolar and unipolar RRAM. Threshold switch-based selector was demonstrated for 64 Mb array. However, One shouldn't forget that the cross-point architecture requires BEOL compatible two terminal selectors like punch-through diode for bipolar RRAM or PIN diode for unipolar RRAM.
Polarity can be either binary or unary. Bipolar effects cause polarity to reverse when switching from low to high resistance (reset operation) compared to switching high to low (set operation). Unipolar switching leaves polarity unaffected, but uses different voltages.
Material systems for resistive memory cells
Multiple inorganic and organic material systems display thermal or ionic resistive switching effects. These can be grouped into the following categories:
- phase-change chalcogenides such as Ge
5 or AgInSbTe
- binary transition metal oxides such as NiO or TiO
- perovskites such as Sr(Zr)TiO
3 or PCMO
- solid-state electrolytes such as GeS, GeSe, SiO
x or Cu
- organic charge-transfer complexes such as CuTCNQ
- organic donor–acceptor systems such as Al AIDCN
- two dimensional (layered) insulating materials like hexagonal boron nitride
Papers at the IEDM Conference in 2007 suggested for the first time that RRAM exhibits lower programming currents than PRAM or MRAM without sacrificing programming performance, retention or endurance. Some commonly cited ReRAM systems are described further below.
At IEDM 2008, the highest-performance RRAM technology to date was demonstrated by ITRI using HfO2 with a Ti buffer layer, showing switching times less than 10 ns and currents less than 30μA. At IEDM 2010, ITRI again broke the speed record, showing <0.3 ns switching time, while also showing process and operation improvements to allow yield up to 100% and endurance up to 10 billion cycles. IMEC presented updates of their RRAM program at the 2012 Symposia on VLSI Technology and Circuits, including a solution with a 500 nA operating current.
ITRI had focused on the Ti/HfO2 system since its first publication in 2008. ITRI's patent 8362454 has since been sold to TSMC; the number of prior licensees is unknown. On the other hand, IMEC focused mainly on Hf/HfO2. Winbond had done more recent work toward advancing and commercializing the HfO2-based RRAM.
Panasonic revealed its TaOx-based ReRAM at IEDM 2008. A key requirement was the need for a high work function metal such as Pt or Ir to interface with the TaOx layer. The change of O content results in resistance change as well as Schottky barrier change. More recently, a Ta2O5/TaOx layer was implemented, which still requires the high work function metal to interface with Ta2O5. This system has been associated with high endurance demonstration (trillion cycles), but products are specified at 100K cycles. Filament diameters as large as ~100 nm have been observed. Panasonic released a 4Mb part with Fujitsu, and is developing 40nm embedded memory with UMC.
On 30 April 2008, HP announced that they had discovered the memristor, originally envisioned as a missing 4th fundamental circuit element by Chua in 1971. On 8 July they announced they would begin prototyping RRAM using their memristors. HP first demonstrated its memristor using TiOx, but later migrated to TaOx, possibly due to improved stability. The TaOx-based device has some material similarity to Panasonic's ReRAM, but the operation characteristics are different. The Hf/HfOx system was similarly studied.
Adesto Technologies' ReRAM is based on filaments generated from the electrode metal rather than oxygen vacancies. The original material system was Ag/GeS2 but eventually migrated to ZrTe/Al2O3. The tellurium filament achieved better stability as compared to silver. Adesto has targeted the ultralow power memory for Internet-of-Things (IoT) applications. Adesto has released products manufactured at Altis foundry and entered into a 45nm foundry agreement with TowerJazz/Panasonic.
Crossbar implements an Ag filament in amorphous Si along with a threshold switching system to achieve a diode+ReRAM. Their system includes the use of a transistor in 1T1R or 1TNR architecture. Crossbar started producing samples at SMIC on the 40nm process in 2017. The Ag filament diameter has been visualized on the scale of tens of nanometers.
Programmable metallization cell
Infineon Technologies calls it conductive-bridging RAM(CBRAM), NEC has a variant called “Nanobridge” and Sony calls their version “electrolytic memory”. New research suggests CBRAM can be 3D printed
ReRam test boards
- Panasonic AM13L-STK2 : MN101LR05D 8-bit MCU with built in ReRAM for evaluation, USB 2.0 connector
Compared to PRAM, RRAM operates at a faster timescale (switching time can be less than 10 ns), while compared to MRAM, it has a simpler, smaller cell structure (less than 8F² MIM stack). A vertical 1D1R (one diode, one resistive switching device) integration can be used for crossbar memory structure to reduce the unit cell size to 4F² (F is the feature dimension). Compared to flash memory and racetrack memory, a lower voltage is sufficient, and hence it can be used in low-power applications. Also, due to its relatively small access latency and high density, RRAM is considered a promising candidate for designing caches.
ITRI has shown that RRAM is scalable below 30 nm. The motion of oxygen atoms is a key phenomenon for oxide-based RRAM; one study indicated that oxygen motion may take place in regions as small as 2 nm. It is believed that if a filament is responsible, it would not exhibit direct scaling with cell size. Instead, the current compliance limit (set by an outside resistor, for example) could define the current-carrying capacity of the filament.
A significant hurdle to realizing the potential of RRAM is the sneak path problem that occurs in larger passive arrays. In 2010, complementary resistive switching (CRS) was introduced as a possible solution to sneak-path current interference. In the CRS approach, the information storing states are pairs of high- and low-resistance states (HRS/LRS and LRS/HRS) so that the overall resistance is always high, allowing larger passive crossbar arrays.
A drawback to the initial CRS solution is the requirement for switching endurance caused by conventional destructive readout based on current measurements. A new approach for a nondestructive readout based on capacity measurement potentially lowers the requirements for both material endurance and power consumption. Bi-layer structure is used to produce the nonlinearity in LRS to avoid the sneak path problem. A single-layer device exhibiting a strong nonlinear conduction in LRS was reported. Another bi-layer structure was introduced for bipolar RRAM to improve the HRS and stability.
Another solution to the sneak current issue is to perform read and reset operations in parallel across an entire row of cells, while using set on selected cells. In this case, for a 3D-RRAM 1TNR array, with a column of N RRAM cells situated above a select transistor, only the intrinsic nonlinearity of the HRS is required to be sufficiently large, since the number of vertical levels N is limited (e.g., N = 8–32), and this has been shown possible for a low-current RRAM system.
- U.S. Patent 6,531,371
- U.S. Patent 7,292,469
- U.S. Patent 6,867,996
- "MN101L ReRAM Embedded MCUs - Panasonic | Mouser". www.mouser.com. Retrieved 2016-06-08.
- H-Y. Lee et al., IEDM 2008.
- Mellor, Chris (7 February 2012), Rambus drops $35m for Unity Semiconductor
- "the new microcontrollers with on-chip non-volatile memory ReRAM" (Press release). Panasonic. May 15, 2012. Retrieved May 16, 2012.
- "Next-gen storage wars: In the battle of RRAM vs 3D NAND flash, all of us are winners" (Press release). PC World. August 9, 2013. Retrieved January 28, 2014.
- Lamb, D R; Rundle, P C (1967). "A non-filamentary switching action in thermally grown silicon dioxide films". British Journal of Applied Physics. 18: 29. Bibcode:1967BJAP...18...29L. doi:10.1088/0508-3443/18/1/306.
- Park, In-Sung; Kim, Kyong-Rae; Lee, Sangsul; Ahn, Jinho (2007). "Resistance Switching Characteristics for Nonvolatile Memory Operation of Binary Metal Oxides". Japanese Journal of Applied Physics. 46 (4B): 2172. Bibcode:2007JaJAP..46.2172P. doi:10.1143/JJAP.46.2172.
- Mehonic, A.; Cueff, S. B.; Wojdak, M.; Hudziak, S.; Jambois, O.; Labbé, C.; Garrido, B.; Rizk, R.; Kenyon, A. J. (2012). "Resistive switching in silicon suboxide films". Journal of Applied Physics. 111 (7): 074507. Bibcode:2012JAP...111g4507M. doi:10.1063/1.3701581.
- Chua, L. O. (2011), "Resistance switching memories are memristors", Applied Physics A, 102 (4): 765–783, Bibcode:2011ApPhA.102..765C, doi:10.1007/s00339-011-6264-9
- Mellor, Chris (10 October 2011), "HP and Hynix to produce the memristor goods by 2013", The Register, retrieved 2012-03-07
- Meuffels, P.; Soni, R. (2012), "Fundamental Issues and Problems in the Realization of Memristors", arXiv:
- Di Ventra, Massimiliano; Pershin, Yuriy V. (2013). "On the physical properties of memristive, memcapacitive and meminductive systems". Nanotechnology. 24 (25): 255201. Bibcode:2013Nanot..24y5201D. PMID 23708238. arXiv: . doi:10.1088/0957-4484/24/25/255201.
- Valov, I.; Linn, E.; Tappertzhofen, S.; Schmelzer, S.; van den Hurk, J.; Lentz, F.; Waser, R. (2013). "Nanobatteries in redox-based resistive switches require extension of memristor theory". Nature Communications. 4: 1771. Bibcode:2013NatCo...4E1771V. PMC . PMID 23612312. doi:10.1038/ncomms2784.
- "the Foresight Institute » Blog Archive » Nanotechnology-based next generation memory nears mass production". Foresight.org. Retrieved 2014-08-13.
- Lanza, Mario (2014). "A Review on Resistive Switching in High-k Dielectrics: A Nanoscale Point of View Using Conductive Atomic Force Microscope". Materials. 7 (3): 2155–2182.
- Lee, D.; Seong, D. J.; Jo, I.; Xiang, F.; Dong, R.; Oh, S.; Hwang, H. (2007). "Resistance switching of copper doped MoO[sub x] films for nonvolatile memory applications". Applied Physics Letters. 90 (12): 122104. Bibcode:2007ApPhL..90l2104L. doi:10.1063/1.2715002.
- "Resistive switching in hafnium dioxide layers: Local phenomenon at grain boundaries". Applied Physics Letters. 101 (19): 193502. 2012-11-05. ISSN 0003-6951. doi:10.1063/1.4765342.
- Shi, Yuanyuan; Ji, Yanfeng; Hui, Fei; Nafria, Montserrat; Porti, Marc; Bersuker, Gennadi; Lanza, Mario (2015-04-01). "In Situ Demonstration of the Link Between Mechanical Strength and Resistive Switching in Resistive Random-Access Memories". Advanced Electronic Materials. 1 (4): n/a–n/a. ISSN 2199-160X. doi:10.1002/aelm.201400058.
- Lanza, Mario (2017). Conductive Atomic Force Microscopy: Applications in Nanomaterials. Berlin, Germany: Wiley-VCH. pp. 10–30. ISBN 978-3-527-34091-0.
- "Advanced Engineering Materials – Wiley Online Library". Aem-journal.com. Retrieved 2014-08-13.
- Y. S. Chen et al., Forming-free HfO2 Bipolar RRAM Device with Improved Endurance and High Speed Operation, VLSI-TSA 2009, p. 37. http://ieeexplore.ieee.org/stamp/stamp.jsp?arnumber=5159281
- M.Balakrishnan et al., A Low Power Non-Volatile Memory Element Based on Copper in Deposited Silicon Oxide, NVMTS 2006, http://ieeexplore.ieee.org/xpls/abs_all.jsp?arnumber=4228446
- S. Sills et al., A Copper ReRAM Cell for Storage Class Memory Applications, Proc. Symp. VLSI Tech. 2014, p. 64.
- I.V. Karpov, D. Kencke, D. Kau, S. Tang and G. Spadini, MRS Proceedings, Volume 1250, 2010
- V. S. S. Srinivasan et al., Punchthrough-Diode-Based Bipolar RRAM Selector by Si Epitaxy," Electron Device Letters, IEEE , vol.33, no.10, pp.1396,1398, Oct. 2012 doi: 10.1109/LED.2012.2209394
- Pan, Chengbin; Ji, Yanfeng; Xiao, Na; Hui, Fei; Tang, Kechao; Guo, Yuzheng; Xie, Xiaoming; Puglisi, Francesco M.; Larcher, Luca (2017-01-01). "Coexistence of Grain-Boundaries-Assisted Bipolar and Threshold Resistive Switching in Multilayer Hexagonal Boron Nitride". Advanced Functional Materials: n/a–n/a. ISSN 1616-3028. doi:10.1002/adfm.201604811.
- Puglisi, F. M.; Larcher, L.; Pan, C.; Xiao, N.; Shi, Y.; Hui, F.; Lanza, M. (2016-12-01). "2D h-BN based RRAM devices". 2016 IEEE International Electron Devices Meeting (IEDM): 34.8.1–34.8.4. doi:10.1109/IEDM.2016.7838544.
- Tsunoda, K.; Kinoshita, K.; Noshiro, H.; Yamazaki, Y.; Iizuka, T.; Ito, Y.; Takahashi, A.; Okano, A.; Sato, Y.; Fukano, T.; Aoki, M.; Sugiyama, Y. (2007). "Low Power and High Speed Switching of Ti-doped NiO ReRAM under the Unipolar Voltage Source of less than 3 V". 2007 IEEE International Electron Devices Meeting. p. 767. ISBN 978-1-4244-1507-6. doi:10.1109/IEDM.2007.4419060.
- H-Y. Lee et al., IEDM 2010.
- L. Goux et al., 2012 Symp. on VLSI Tech. Dig. of Tech. Papers, 159 (2012).
- Y. Y. Chen et al., IEDM 2013.
- C-H. Ho et al., 2016 Symposium on VLSI Technology.
- Z. Wei et al., IEDM 2008.
- Y. Hayakawa et al., 2015 Symposium on VLSI Technology.
- M-J. Lee et al., Nat. Mat. 10, 625 (2011).
- Panasonic ReRAM-based product description
- Z. Wei, IMW 2013.
- Fujitsu announces 4Mb ReRAM
- Panasonic and UMC announce ReRAM development
- EETimes.com – Memristors ready for prime time
- D. B. Strukov, Nature 453, 80 (2008).
- J. P. Strachan et al., IEEE Trans. Elec. Dev. 60, 2194 (2013).
- Comparison of Pt/TiOx/Pt vs Pt/TaOx/TaOy/Pt
- S. Kumar et al., ACS Nano 10, 11205 (2016).
- J. R. Jameson et al., IEDM 2013.
- D. Kanter, "Adesto Targets IoT Using CBRAM, The Linley Group Microprocessor Report, Feb 2016.
- Altis CBRAM for Adesto
- Adesto/TPsco agreement
- Y. Dong et al., Nano. Lett. 8, 386 (2008).
- S. H. Jo et al., ASPDAC 2015.
- Crossbar sampling 40nm at SMIC
- TEMs of Ag filament
- Fully inkjet printed flexible resistive memory -AIP Scitation
- Mass Producing Printed Electronics -Engineering.com
- Zhang, Yang; Duan, Ziqing; Li, Rui; Ku, Chieh-Jen; Reyes, Pavel I; Ashrafi, Almamun; Zhong, Jian; Lu, Yicheng (2013). "Vertically integrated ZnO-Based 1D1R structure for resistive switching". Journal of Physics D: Applied Physics. 46 (14): 145101. Bibcode:2013JPhD...46n5101Z. doi:10.1088/0022-3727/46/14/145101.
- "A Survey Of Architectural Approaches for Managing Embedded DRAM and Non-volatile On-chip Caches", Mittal et al., TPDS, 2015.
- Y.-S. Chen et al., IEDM 2009.
- New Non-Volatile Memory Workshop 2008, Hsinchu, Taiwan.
- Cen, C.; Thiel, S.; Hammerl, G.; Schneider, C. W.; Andersen, K. E.; Hellberg, C. S.; Mannhart, J.; Levy, J. (2008). "Nanoscale control of an interfacial metal–insulator transition at room temperature". Nature Materials. 7 (4): 298. Bibcode:2008NatMa...7..298C. PMID 18311143. doi:10.1038/nmat2136.
- I. G. Baek et al.,IEDM 2004.
- Lin, Chih-Yang; Wu, Chen-Yu; Wu, Chung-Yi; Hu, Chenming; Tseng, Tseung-Yuen (2007). "Bistable Resistive Switching in Al2O3 Memory Thin Films". Journal of the Electrochemical Society. 154 (9): G189. doi:10.1149/1.2750450.
- Linn, Eike; Rosezin, Roland; Kügeler, Carsten; Waser, Rainer (2010). "Complementary resistive switches for passive nanocrossbar memories". Nature Materials. 9 (5): 403. Bibcode:2010NatMa...9..403L. PMID 20400954. doi:10.1038/nmat2748.
- Tappertzhofen, S; Linn, E; Nielen, L; Rosezin, R; Lentz, F; Bruchhaus, R; Valov, I; Böttger, U; Waser, R (2011). "Capacity based nondestructive readout for complementary resistive switches". Nanotechnology. 22 (39): 395203. Bibcode:2011Nanot..22M5203T. PMID 21891857. doi:10.1088/0957-4484/22/39/395203.
- Joshua Yang, J.; Zhang, M.-X.; Pickett, Matthew D.; Miao, Feng; Paul Strachan, John; Li, Wen-Di; Yi, Wei; Ohlberg, Douglas A. A.; Joon Choi, Byung; Wu, Wei; Nickel, Janice H.; Medeiros-Ribeiro, Gilberto; Stanley Williams, R. (2012). "Engineering nonlinearity into memristors for passive crossbar applications". Applied Physics Letters. 100 (11): 113501. Bibcode:2012ApPhL.100k3501J. doi:10.1063/1.3693392.
- Mehonic, Adnan; Cueff, Sébastien; Wojdak, Maciej; Hudziak, Stephen; Labbé, Christophe; Rizk, Richard; Kenyon, Anthony J (2012). "Electrically tailored resistance switching in silicon oxide". Nanotechnology. 23 (45): 455201. Bibcode:2012Nanot..23S5201M. PMID 23064085. doi:10.1088/0957-4484/23/45/455201.
- Zhang, Yang; Duan, Ziqing; Li, Rui; Ku, Chieh-Jen; Reyes, Pavel; Ashrafi, Almamun; Lu, Yicheng (2012). "FeZnO-Based Resistive Switching Devices". Journal of Electronic Materials. 41 (10): 2880. Bibcode:2012JEMat..41.2880Z. doi:10.1007/s11664-012-2045-2.
- H. S. Yoon et al., Vertical cross-point resistance change memory for ultra-high density non-volatile memory applications, Proc. Symp. VLSI Tech. 2009, pp. 26–27. http://ieeexplore.ieee.org/xpl/login.jsp?tp=&arnumber=5200621&url=http%3A%2F%2Fieeexplore.ieee.org%2Fxpls%2Fabs_all.jsp%3Farnumber%3D5200621
- F. T. Chen et al., Write Scheme Allowing Reduced LRS Nonlinearity Requirement in a 3D-RRAM Array With Selector-Less 1TNR Architecture, IEEE Elec. Dev. Lett. vol. 35, 223 (2014). http://ieeexplore.ieee.org/xpl/articleDetails.jsp?arnumber=6701133
- Poremba et al., "DESTINY: A Tool for Modeling Emerging 3D NVM and eDRAM caches", DATE, 2015.